Contents lists available atScienceDirect
An overview of water electrolysis technologies for green hydrogen production
S. Shiva Kumara
, Hankwon Lima,b,c,∗
aCarbon Neutrality Demonstration and Research Center, Ulsan National Institute of Science and Technology, 50 UNIST-gil, Eonyang-up, Ulju-gun, Ulsan 44919, Republic of Korea
bGraduate School of Carbon Neutrality, Ulsan National Institute of Science and Technology, 50 UNIST-gil, Eonyang-up, Ulju-gun, Ulsan 44919, Republic of Korea
cSchool of Energy and Chemical Engineering, Ulsan National Institute of Science and Technology, 50 UNIST-gil, Eonyang-up, Ulju-gun, Ulsan 44919, Republic of Korea
a r t i c l e i n f o
Received 21 July 2022
Received in revised form 21 September 2022 Accepted 6 October 2022
Available online xxxx Keywords:
Green hydrogen production Alkaline water electrolysis Anion exchange membrane water electrolysis
Proton exchange membrane water electrolysis
Solid oxide water electrolysis
a b s t r a c t
Decarbonizing the planet is one of the major goals that countries around the world have set for 2050 to mitigate the effects of climate change. To achieve these goals, green hydrogen that can be produced from the electrolysis of water is an important key solution to tackle global decar- bonization. Consequently, in recent years there is an increase in interest towards green hydrogen production through the electrolysis process for large-scale implementation of renewable energy- based power plants and other industrial, and transportation applications. The main objective of this study was to provide a comprehensive review of various green hydrogen production technologies especially on water electrolysis. In this review, various water electrolysis technologies and their techno-commercial prospects including hydrogen production cost, along with recent developments in electrode materials, and their challenges were summarized. Further some of the most successful results also were described. Moreover this review aims to identify the gaps in water electrolysis research and development towards the techno-commercial perspective. In addition, some of the commercial electrolyzer performances and their limitations also were described along with possible solutions for cost-effective hydrogen production Finally, we outlined our ideas, and possible solutions for driving cost-effective green hydrogen production for commercial applications. This information will provide future research directions and a road map for the development/implementation of commercially viable green hydrogen projects.
©2022 The Author(s). Published by Elsevier Ltd. This is an open access article under the CC BY license (http://creativecommons.org/licenses/by/4.0/).
1. Introduction... 13794
2. Hydrogen production... 13794
2.1. Significant role of green hydrogen in energy transition... 13795
3. Water electrolysis... 13795
3.1. Alkaline water electrolysis ... 13796
3.1.1. Working principle of alkaline water electrolysis... 13796
3.1.2. Cell components of alkaline water electrolysis... 13796
3.1.3. Research and development of alkaline water electrolysis... 13797
3.2. Anion exchange membrane (AEM) water electrolysis... 13798
3.2.1. Working principle of AEM water electrolysis... 13799
3.2.2. Cell components of AEM water electrolysis... 13799
3.2.3. Research and development of AEM water electrolysis... 13800
3.3. PEM water electrolysis... 13802
3.3.1. Working principle of pem water electrolysis... 13803
∗ Corresponding author at: Carbon Neutrality Demonstration and Research Center, Ulsan National Institute of Science and Technology, 50 UNIST-gil, Eonyang-up, Ulju-gun, Ulsan 44919, Republic of Korea.
E-mail addresses: firstname.lastname@example.org(S. Shiva Kumar),email@example.com(H. Lim).
2352-4847/©2022 The Author(s). Published by Elsevier Ltd. This is an open access article under the CC BY license (http://creativecommons.org/licenses/by/4.0/).
due to an increase in population and standards of living, apart from the industrial growth of developing countries (Ibrahim, 2012;Mostafa et al.,2019). Inductively the global primary energy supply was 14,410 MTOE in 2019 (IEA,2019a). According to the International energy agency’s prediction, the global energy de- mand will be increased by 50% in 2030 (EIA,2016). To date, more than 95% of this huge energy demand is fulfilled by using fossil fu- els, however, the use of fossil fuels releases a high concentration of greenhouse gas emissions consequently increasing the global warming and environmental pollution (Sazal, 2020; Lee et al., 2018). Therefore, the rapid development of alternative green en- ergy technologies is essential to meet global energy demands and sustainable development. In this context, the ‘Paris Agreement’
was framed and approved by 196 parties at the 21st conference of the parties (COP 21) in 2015, which aims to respond to the global warming actively by preventing a global temperature rise below 1.5◦C (Jacquet and Jamieson,2016). In addition, many countries have focused on introducing environmentally friendly energy policies for a sustainable environment and decarbonization. For example, South Korea announced the 2nd Climate Change Re- sponse Master Plan in 2019 to reduce greenhouse gas emissions from 709.1 million tons in 2017 to 536 million tons by 2030 for a sustainable and low-carbon green society (Lee et al.,2020).
Thus, globally various research institutions/organizations have moved towards the development of innovative technologies that can utilize renewable sources for generating green energy and fuels. Hydrogen is one such promising environmentally friendly renewable energy carrier and it is the most abundant element in the universe (Immanuel and Dmitri,2018;Pinsky et al.,2020;
Dawood et al., 2020). The hydrogen atom is composed of one proton and one electron, making it the lightest element in the universe, and having unique properties like high energy den- sity (120 MJ/kg) and lower volumetric energy density (8 MJ/L).
However, it is not readily available directly on the earth, it is available in chemically combined forms of water, fossil fuels, and biomass. Hence the main challenge is to separate hydrogen from the naturally occurring compounds efficiently and economically.
2. Hydrogen production
Hydrogen can be produced from various sources of raw mate- rials including renewable and non-renewable sources which are around 87 million tons/year (Dawood et al.,2020;Milani et al., 2020). However, as of 2020, most of the hydrogen (95%) was produced from non-renewable fossil fuels especially steam re- forming of natural gas, emitting 830 million tons/year of CO2and the rest of the hydrogen was produced from renewable resources including water electrolysis (Mosca et al.,2020;IEA,2019b). The
drogen production technology, energy source, and environmental impact (Noussan et al.,2021;Ajanovic et al.,2022), as shown in Table 1. The blue hydrogen is produced from the steam reform- ing of natural gas. During this process, natural gas is split into hydrogen (H2) and carbon dioxide (CO2), the produced CO2is cap- tured (85%–95%) and stored underground using industrial carbon capture and storage techniques and some of the generated CO2 cannot be captured. In addition, long-term impacts of storage are uncertain, and leakage can still negatively affect the environment and climate (Hermesmann and Muller,2022;Navas-Anguita et al., 2021). The gray hydrogen is produced from non-renewable fossil fuels such as natural gas or coal by steam reforming/auto-thermal reforming process, this process is similar to the blue hydrogen process, but the produced CO2is not being captured, it is directly released into the atmosphere (Nikolaidis and Poullikkas,2017).
Brown hydrogen is most abundant in use today, which is pro- duced from hydrocarbon-rich feedstock (brown coal or methane) via the gasification process. But as a result, every tone of brown hydrogen releases 10–12 tons of CO2 into the atmosphere. The black hydrogen is produced from coal gasification, during this coal gasification process syngas are produced from the gasifier and the hydrogen can be separated from the other gases using absorbers or special membranes and the remaining gases can be released into the atmosphere (IRENA,2020a;IEA,2019b). Green hydrogen is produced from renewable water and electricity by electrolysis process, in this process water is split into hydrogen (H2) and oxygen (O2) under the influence of electricity with zero carbon emissions (Carmo et al.,2013).
In the transition towards global decarbonization, nowadays renewable-powered green hydrogen generation is one way that is increasingly being considered as a means of reducing greenhouse gas emissions and environmental pollution (Yue et al.,2021;Bur- ton et al.,2021). Hence, there is an increasing interest to make the production and utilization of this green hydrogen more scalable and versatile process. Water electrolysis is a key technology for splitting water into hydrogen and oxygen by using renewable en- ergy (solar, wind) (Ibrahim,2012;Burton et al.,2021). Solar and wind energies are prepared and well suitable renewable power sources for hydrogen production through water electrolysis due to their widespread power distribution (Wang et al.,2014). The combination of renewable energy with water electrolysis is par- ticularly more advantageous because surplus electrical energy can be stored chemically in the form of hydrogen to balance the discrepancy between energy demand and production (Brauns and Thomas,2020). Further, the produced hydrogen and oxygen can be directly used for the transportation and industrial sector as primary energy sources. Hydrogen is not only a primary energy source it is an energy carrier that can be directly used in fuel cell vehicles and the industrial sector. Moreover, hydrogen can also
Fig. 1. Major hydrogen production methods and applications. . (For interpretation of the references to color in this figure legend, the reader is referred to the web version of this article.)
Hydrogen color shades and their Technology, cost, and CO2emissions.
be used as a feedstock in chemical and petrochemical industries to produce ammonia and synthetic fuels (Jovan and Dolanc,2020;
Shiva Kumar and Himabindu,2019a;Shiva Kumar et al.,2019b).
Apart from that, another advantage of hydrogen as an energy carrier is the increased efficiency of hydrogen storage systems when compared to batteries.
2.1. Significant role of green hydrogen in energy transition Green hydrogen is widely viewed as a promising fuel for future sustainable development and energy transition due to fact that green hydrogen can be produced from water and renewable en- ergy sources through the electrolysis process, in this process there are no greenhouse gas emissions. Therefore, green hydrogen is increasingly being promoted to address climate change issues and meet the global net-zero challenges. Moreover, global demand for green hydrogen and its applications is expected to increase exponentially over the next decade. Fortunately, globally some projects are already underway to produce green hydrogen from renewable energy sources like wind and solar (IEA,2021).
3. Water electrolysis
Water electrolysis is one such electrochemical water splitting technique for green hydrogen production with the help of elec- tricity, which is emission-free technology. The basic reaction of water electrolysis is as follows in Eq.(1).
1 H2O+Electricity (237.2 kJ mol−1)+Heat (48.6 kJ mol−1)
The above reaction (Eq.(1)) requires 1.23 V theoretical thermo- dynamic cell voltage to split the water into hydrogen and oxygen at room temperature. However, experimentally the required cell voltage for efficient water splitting is 1.48 V. The additional voltage is required to overcome the kinetics and ohmic resis- tance of the electrolyte and cell components of the electrolyzer (Shiva Kumar and Himabindu,2020;Lee et al.,2021b;Lim et al., 2021).
Past two centuries, water electrolysis is a well-known tech- nology for green hydrogen production. However, globally only 4% of hydrogen (65 million tons) can be produced from water electrolysis due to economic issues, with most of this hydrogen being produced as a by-product from the Chlor-alkali industry (Yu et al.,2018;Hall et al.,2020;Yodwong et al.,2020). The largest electrolysis plant (135 MW/30,000 N m3/h) has been deployed for the fertilizer industry (Bertuccioli et al.,2014a,b). Since the 18th century, water electrolysis technologies are being continuously developed and used in industrial applications, during this journey different trends have affected its development, with this split into roughly five generations. Each generation of water elec- trolysis and their challenges, technological breakthroughs, and significance are shown inFig. 2.
During these developments, four types of water electrolysis technologies were introduced based on their electrolyte, operat- ing conditions, and their ionic agents (OH−, H+, O2−), such as (i) Alkaline water electrolysis (ii) AEM water electrolysis
Fig. 2. Generations of water electrolysis development (IRENA,2020b).
(iii) PEM water electrolysis and (iv) Solid oxide water electrol- ysis. However, the operating principles are the same for all the cases (Shiva Kumar and Himabindu, 2019a). The four types of water electrolysis technologies and their characteristics along with advantages, disadvantages were described in the following subsections andTables 2&3.
3.1. Alkaline water electrolysis
Alkaline water electrolysis is well established mature technol- ogy for industrial hydrogen production up to the multi-megawatt range in commercial applications across the globe (Kuckshinrichs et al., 2017). The alkaline water electrolysis phenomenon was first introduced by Troostwijk and Diemann in the year 1789.
After several developments in the year of 1939, the first industrial large-scale alkaline water electrolyzer plant with the capacity of 10,000 N m3 H2h−1 went into operation (Diogo et al.,2013).
In later early 19th century, more than 400 industrial alkaline electrolyzer units were successfully installed and operated for industrial applications (Grigoriev et al.,2020). However, the alka- line water electrolyzer operates at lower temperatures (30–80◦C) with a concentrated alkaline solution (5M KOH/NaOH). Moreover, in alkaline water electrolyzer nickel (Ni) coated stainless steel electrodes and asbestos/ZrO2-based diaphragms are used as a separator (Shiva Kumar et al.,2018a,b,c,d,2017). The ionic charge carrier is hydroxyl ion (OH−) with KOH/NaOH and water perme- ating through the porous structure of the diaphragm to provide the functionality of the electrochemical reaction (Shiva Kumar et al., 2017; Lee et al., 2021a). The alkaline water electrolysis is a favorable system design for large-scale applications. Today, the investment cost of alkaline water electrolysis is USD 500–
1000/kW, and the lifetime of the system is 90,000 h (Bertuccioli et al.,2014a,b; Schmidt et al.,2017). However, the major chal- lenge associated with alkaline water electrolysis is limited current densities (0.1–0.5 A/cm2) due to moderate OH− mobility, and usage of corrosive (KOH) electrolytes (IRENA,2020a). Due to the high sensitivity of the KOH electrolyte to ambient CO2 and the subsequent salt formation of K2CO3, the resulting decrease in the
number of hydroxyl ions and ionic conductivity. In addition, the salt of K2CO3 close the pores of the anode gas diffusion layer which subsequently decreases the ion transferability through the diaphragm and consequent reduction of hydrogen production.
Apart from that, the alkaline water electrolysis produces low purity (99.9%) of gasses (Hydrogen and Oxygen) due to the ex- isting diaphragm does not completely prevent the crossover of the gases from one half-cell to the other.
3.1.1. Working principle of alkaline water electrolysis
Alkaline water electrolysis is an electrochemical water split- ting techniques in the presence of electricity. The electrochemical water splitting consists of two individual half-cell reactions such as hydrogen evolution reaction (HER) at the cathode and oxygen evolution reaction (OER) at the anode. During the alkaline elec- trolysis process, initially at the cathode side two moles of alkaline solution are reduced to produce one mole of hydrogen (H2) and two moles of hydroxyl ions (OH−), the produced H2 can be eliminated from the cathodic surface and the remaining hydroxyl ions (OH−) are transferred under the influence of electric circuit between anode and cathode through the porous separator to the anode side. At the anode, the hydroxyl ions (OH−) are discharged to produce the1/2molecule of oxygen (O2) and one molecule of water (H2O), as shown inFig. 3.
3.1.2. Cell components of alkaline water electrolysis
The major alkaline water electrolysis cell components are diaphragms/separators, current collectors (gas diffusion layer), separator plates (bipolar plates), and end plates respectively. In general, Asbestos/Zirfon/Nickel coated perforated stainless-steel diaphragms are used as separators in alkaline water electrol- ysis (David et al., 2019; Shiva Kumar et al., 2017). The nickel mesh/foam is used as gas diffusion layers and stainless steel/nickel-coated stainless steel separator plates are used as bipolar and end plates respectively.
Technical characteristics of typical water electrolysis technologies (IRENA,2020b).
Alkaline AEM PEM Solid Oxide
Anode reaction 2OH−→H2O+ 12O2+2e− 2OH−→H2O+ 12 O2+2e− H2O→2H++ 12O2+2e− O2−→ 12 O2+2e− Cathode Reaction 2 H2O+2e−→H2+2OH− 2 H2O+2e−→H2+ 2OH− 2H++2e−→H2 H2O+2e−→H2+O2− Overall cell H2O→H2+ 12 O2 H2O→H2+12 O2 2H2O→H2+12 O2 H2O→H2+ 12 O2
Electrolyte KOH/NaOH (5M) DVB polymer support with 1
Solid polymer electrolyte (PFSA)
Yttria stabilized Zirconia (YSZ)
Separator Asbestos/Zirfon/Ni Fumatech, Nafion® Solid electrolyte YSZ
Electrode/Catalyst (Hydrogen side)
Nickel coated perforated stainless steel
Nickel Iridium oxide Ni/YSZ
Electrode/Catalyst (Oxygen side)
Nickel coated perforated stainless steel
Nickel or NiFeCo alloys Platinum carbon Perovskites (LSCF, LSM) (La,Sr,Co,FE) (La,Sr,Mn) Gas Diffusion layer Nickel mesh Nickel foam/carbon cloth Titanium mesh/carbon cloth Nickel mesh/foam Bipolar Plates Stainless steel/Nickel coated
Stainless steel/Nickel coated stainless steel
Platinum/Gold-coated Titanium or Titanium
Cobalt coated stainless steel
Nominal current density
0.2–0.8 A/cm2 0.2–2 A/cm2 1–2 A/cm2 0.3–1 A/cm2
Voltage range (limits) 1.4–3 V 1.4–2.0 V 1.4–2.5 V 1.0–1.5 V
70–90◦C 40–60◦C 50–80◦C 700–850◦C
Cell pressure <30 bar <35 bar <70 bar 1 bar
H2 purity 99.5–99.9998% 99.9–99.9999% 99.9–99.9999% 99.9%
Efficiency 50%–78% 57%–59% 50%–83% 89% (laboratory)
Lifetime (stack) 60 000 h >30 000 h 50 000–80 000 h 20 000 h
Development status Mature R & D Commercialized R & D
Electrode area 10 000–30 000 cm2 <300 cm2 1500 cm2 200 cm2
Capital costs (stack) minimum 1 MW
USD 270/kW Unknown USD 400/kW >USD 2000/kW
Capital costs (stack) minimum 10 MW
USD 500–1000/kW Unknown USD 700–1400/kW Unknown
Advantages and disadvantages of typical water electrolysis technologies.
Electrolysis technology Advantages Disadvantages
Alkaline water electrolysis
•Well established Technology
•Commercialized for industrial applications
•Noble metal-free electrocatalysts
•Relatively low cost
•Limited current densities
•Crossover of the gasses
•High concentrated (5M KOH) liquid electrolyte
AEM water electrolysis •Noble metal-free electrocatalysts
•Low concentrated (1M KOH) liquid electrolyte.
PEM water electrolysis •Commercialized technology
•Operates higher current densities
•High purity of the gases
•Compact system design
•Cost of the cell components
•Noble metal electrocatalysts
Solid oxide water electrolysis
•High working temperature
3.1.3. Research and development of alkaline water electrolysis Alkaline water electrolysis is a mature and well-established technology up to the multi-megawatt scale and globally number of manufacturers are successfully deployed and used for indus- trial applications (IRENA,2020b; IEA, 2021), some of the com- mercial alkaline water electrolyzers and their manufacturers are listed inTable 4. However, some improvements are still needed in this technology such as increase in the current density and reduce the crossover of the gasses. To achieve these challenges, new electrode materials and separators need to be developed.
Moreover, an alkaline water electrolyzer can be integrated with renewable energy (solar, wind) sources which can be more ben- eficial for reducing the capital cost. In this direction, some of the research institutes/organizations are still actively working on
increasing the efficiency and reducing hydrogen production cost.
For example, Liu et al. (2020) reported heterojunction hybrid structures of MoS2@Ni0.96S as a low-cost and noble metal-free bifunctional electrocatalysts for OER and HER in alkaline media.
The developed MoS2@Ni0.96S-1 electrocatalyst exhibited a signifi- cantly lower overpotential of 104 mV at 10 mA cm−2towards the HER and OER overpotential of 182 mV at 10 mA cm−2with the highest HER and OER activity. Additionally, achieved a lower cell voltage of 1.86 V for the overall water splitting and demonstrated superior stability during the continuous operation of 15 h. This improvement is mainly due to strong integration between ultra- thin MoS2nanosheets with non-stoichiometric Ni0.96S nanocrys- tals, exposure of more active sites, and presence of abundant heterojunction interfaces within MoS2@Ni0.96S-1h. Qazi et al.
Fig. 3. Schematic illustration of alkaline water electrolysis working principle.
(2021) developed an efficient bifunctional nano heterostructure electrocatalyst of NiCo-NiCoO2@Cu2O@CF for overall water split- ting and studied their performance in 1M KOH solution. As prepared NiCo-NiCoO2@Cu2O@CF electrocatalyst has shown im- proved electrochemical performance towards the HER and OER in alkaline media with a lower overpotential of 133 and 327 mV to achieve a current density of 10 mA cm2 with a small Tafel slope of 119 and 118 mV dec−1 for HER and OER respectively.
In addition, experimentally studied their performance through single-cell electrolysis process using NiCo-NiCoO2@Cu2O@CF as a bifunctional electrocatalyst for both HER and OER. The re- sults showed better electrochemical performance than the other non-noble metal electrocatalysts, the attained cell voltage of 1.69 V to reach the current density ≥10 mA cm−2. Further, the developed electrocatalyst was stable during the continuous electrolysis process of 12 h in a strong alkaline solution due to the robust mechanical adhesion between NiCo-NiCoO2nanopar- ticles. The better performance was achieved by the small size of NiCo-NiCoO2nano heterostructures uniformly distributed on the oxidized surface of copper foam enabling them to maximum uti- lization active sites during the electrochemical reactions.Xu et al.
(2022) developed a highly efficient bifunctional electrocatalyst of 2D metal–organic framework (MOF)-derived NiCoP nanoflakes (NiCo(nf)-P) for overall water splitting in alkaline media. The developed electrocatalyst performance were studied by three- electrode cell assembly with linear sweep voltammetry (LSV) method at the potential cycling rate of 2 mV s−1 in a 1M KOH electrolyte solution. The developed NiCo(nf)-P was shown better electrocatalytic activity with a lower onset potential of 37 mV and 1.435 V than commercial 5% Pt/C (43 mV) and IrO2(1.504 V) at the current density of 100 mV cm−2 towards the HER and OER.
In addition, NiCo(nf)-P was shown lower overpotential of 119 mV and 315 mV than commercial 5% Pt/C (291 mV) and IrO2(400) to achieve the current density of 100 mV cm−2towards the HER and OER. The Tafel slope also potentially lower for NiCo(nf)-P (112 mV dec−1) and 66 mV dec−1than commercial 5% Pt/C (164 mV dec−1) and IrO2(88 mV dec−1), which indicates the rapid charge transfer across the electrocatalytic interfaces of as developed NiCo(nf)-P.
Further, the developed NiCo(nf)-P electrocatalyst stability studies were carried out at different current densities of 100, 500, and 1000 mA cm−2 towards the HER and OER using chronopoten- tiometric (V-t) measurements. The, attained results show the stable electrochemical performance during the 30 h of continuous operation, as shown inFig. 4. Moreover, the developed NiCo(nf)- P electrocatalyst HER and OER performance also were studied in alkaline electrolyzer, it shows the excellent electrocatalytic
activity with a lower cell voltage of 1.94 V at the operating current density of 1 A cm−2.
Further, Jin et al. (2021) have synthesized N-doped carbon supported Ni-Mo-O/Ni4Mo nanointerface electrocatalyst (Ni-Mo- O/Ni4Mo@NC) by electrodeposition–calcination–electrodeposition techniques and studied their electrocatalytic activity towards the hydrogen evolution reaction in alkaline solution (1M KOH).
The synthesized Ni-Mo-O/Ni4Mo@NC electrocatalyst has shown a higher electrocatalytic activity with a lower overpotential of 61 mV at a geometric current density of 10 mA cm−2, which is 50% lower than that of Ni-Mo-O (120 mV) due to the introduction of N-doped carbon layers. Also, studies in neutral conditions (1M PBS solution) Ni-Mo-O/Ni4Mo@NC shows an overpotential of <
60 mV, which is lower than that of Ni-Mo-O (∼100 mV). The Tafel slope of Ni-Mo-O/Ni4Mo@NC is determined to be 99 mV dec−1, which is relatively lower than that of Ni-Mo-O (135 mV dec−1).Lv et al. (2021) introduced multi-heterostructure inter- faces and 3D porous structures of Co2P/N@Ti3C2Tx@NF as an efficient HER electrocatalyst for alkaline media. Initially, CPN@TC with multi-heterostructure interfaces were fabricated on the sur- face of MXene (Ti3C2Tx)-modified NF by a two-step electrode- position method and subsequent nitriding process. The prepared Co2P/N@Ti3C2Tx@NF electrocatalyst performance was studied in 1M KOH solution, the results exhibited an outstanding HER per- formance with an overpotential of only 15 mV at 10 mA cm−2 and a small Tafel slope of 30 mV dec−1, as shown in Fig. 5.
In addition, shown superior stability during the 3000 cycles of CV tests and only 20 mV shifting can be at the current density of 100 mA cm−2. In addition, water dissociation (∆G∗H2O) and hydrogen adsorption (∆G∗H) energies were calculated by DFT (density functional theory) for different materials. According to the DFT calculations, the prepared CPN@TC has strongest binding energy of−0.822 eV, which is favorable for the HER reactions.
Also, the prepared CPN@TC possesses an H* adsorption energy with the closest value to zero, which is generally considered to be the best electrocatalyst.
3.2. Anion exchange membrane (AEM) water electrolysis
AEM water electrolysis is a developing technology for green hydrogen production. Over the past few years, many research organizations/institutions are actively working in the develop- ment of AEMWE due to its low cost and high performance com- pared to the other conventional electrolysis technologies. The first journal publication on AEMWE was by We and Scott in 2011 latter many researchers are contributing to the development
Fig. 4. Electrocatalytic activity of as synthesized electrocatalysts LDH(NS), NiCo(NS)-P, MOF(nf), NiCo(nf)-P, NiCo(NR)-P, and commercial 5% Pt/C and IrO2. (a) HER LSV curves, (b) HER overpotentials at different current densities of 100, 500, and 1000 mA cm−2and (c) HER Tafel slopes. (d) OER LSV curves, (e) OER overpotentials at different current densities of 100, 500, and 1000 mA cm−2(f) OER Tafel slopes (g, h) NiCo(nf)-P electrocatalyst HER and OER stability studies (V-t curves) at different current densities of 100, 500, and 1000 mA cm−2(i) LSV curves of NiCo(nf)-P and NiCo(nf)-P; Commercial IrO2and 5% Pt/C for overall water splitting. The inset is the V-t curves of NiCo(nf)-P at current densities of 100, 500, and 1000 mA cm−2towards overall water splitting (Xu et al.,2022).
of AEMWE (Wang et al., 2020a,b). The AEM water electrolysis technology is similar to conventional alkaline water electrolysis (Miller et al.,2020). However, the main difference between alka- line and AEM water electrolysis is the replacement of the conven- tional diaphragms (asbestos) with an anion exchange membrane (quaternary ammonium ion exchange membranes) in alkaline water electrolysis. AEM water electrolysis offers several advan- tages such as cost-effective transition metal catalysts being used instead of noble metal catalysts, distilled water/low concentrated alkaline solution (1M KOH) can be used as electrolyte instead of high concentrated (5 KOH solution) (Henkensmeier et al.,2021).
Despite the significant advantages, AEMWE still required further investigations/improvements towards the MEA stability and cell efficiency which are more essential for large-scale or commercial applications. As of now, the reported stability is 2000 h with Sustain ion and 1000 h for Fumatech (A 201 and FAA3-50), and
>35,000 h for Enapter multicore AEM electrolyzer (Pavel et al., 2014;Carbone et al.,2020;Enapter, Germany).
3.2.1. Working principle of AEM water electrolysis
AEM water electrolysis is one of the electrochemical water splitting techniques with the help of an anion exchange mem- brane and electricity. The electrochemical reaction consists of two half-cell reactions they are hydrogen evolution reaction (HER)
and oxygen evolution reaction (OER). Initially, at the cathode side, the water molecule is reduced to generate hydrogen (H2) and hy- droxyl ions (OH−) by the addition of two electrons. The hydrogen is released from the surface of cathode and the hydroxyl ions (OH−) are diffused through the ion exchange membrane to the anode side by the positive attraction of the anode, while the elec- trons are transported through the external circuit to the anode. At the anode side, the hydroxyl ions recombine as a water molecules and oxygen by losing electrons. The produced oxygen is released from the anode. The basic principle and half-cell reactions of AEM water electrolysis as shown inFig. 6.
3.2.2. Cell components of AEM water electrolysis
Generally, AEM water electrolysis cell components are mem- brane (separator), electrode materials current collectors (gas dif- fusion layer), separator plates (bipolar plates), and end plates respectively. Typical anion exchange membranes are quaternary ammonium ion exchange membranes i.e., Sustanion®, Fumasep, Fumatech respectively. Commonly used anode and cathode elec- trode materials are transition metal based electrocatalysts espe- cially Nickel and NiFeCo alloy materials respectively. The nickel foam/porous nickel mesh and carbon cloth are used as anode and cathode gas diffusion layers. Stainless steel and nickel-coated
Fig. 5. (a) HER Polarization curves of CPN@TC, CP@TC, CP@NF, NF, CPN@NF and TC@NF (b) Tafel plots (c) comparison of CPN@TC with reported electrocatalysts (d) Long-term chronopotentiometry results of CPN@TC at different current densities (−10,−20,−40,−60,−80 mA cm−2) and durability polarization curves for CPN@TC before and after 3000 cycles (e) Calculated H2O adsorption energy. (f) H* adsorption energy (Lv et al.,2021).
Fig. 6. Schematic view of AEM water electrolysis working principle.
stainless steel separator plates are used as bipolar and end plates respectively (Pushkareva et al.,2020).
3.2.3. Research and development of AEM water electrolysis AEM water electrolysis technology is under the developmental stage up to the kW scale. Globally, several research organiza- tions/institutions are actively working on the development of AEM water electrolyzers, some of the AEM water electrolyzer manufacturers/developers are listed in Table 4. However, sev- eral innovations/improvements are still needed to scale up this technology for commercial applications. The major challenges are limited stability (at present 35,000 h and targeted stability of 1,00,000 h) and high hydrogen production cost, present hydrogen production cost is USD 1279 kW/H2 (2020), and the targeted cost reduction of USD ≤300 kW/H2 (2050) (Ionomr,2020). To achieve these targets, the existing challenges need to be ad- dressed economically to commercialize for market applications.
In this direction,Thangavel et al.(2021) developed a 3D oxygen evolution electrode via electrochemical integration of amorphous
NiFeOOH on activated carbon fiber paper (CFP) by single-step co-electrodeposition techniques and their performance in 1M KOH solution. The developed 3D-a-NiFeOOH/N-CFP electrode has shown a better electrochemical performance with an overpoten- tial of only 170 mV at a current density of 10 mA cm−2 and a smaller Tafel slope of 39 mV dec−1 and outstanding stability in 1M KOH solution, as shown inFig. 7. This enhancement is due to the unique 3D structures with increased active sites and the enhanced electrical conductivity that helps enhance the OER ki- netics and mass transport properties. In addition, Fe-doping plays a key role in enhanced OER activity of 3D-a-NiFeOOH/N-CFP. Ad- ditionally, the developed 3D-a-NiFeOOH/N-CFP electrode OER ac- tivity was studied in a single-cell alkaline AEM water electrolyzer with ultra-pure water and compared with commercial IrO2elec- trodes under similar experimental conditions. Impressively, the developed 3D-a-NiFeOOH/N-CFP electrode exhibits superior elec- trochemical performance to commercial IrO2 electrodes, the at- tained cell voltage of 1.88 V than commercial IrO2 2.08 V at
Fig. 7. (a) Schematic representation of 3D-a-NiFeOOH/N-CFP synthesis procedure. (b) LSV curves of various synthesized electrodes in 1 M KOH solution at a scan rate of 1 mV s−1. (c) OER Tafel plots (d) Schematic view of the alkaline AEM water electrolyzer cell. (e) Current–Voltage polarization curves of the alkaline AEM water electrolysis fabricated with 3D-a-NiFeOOH/N-CFP and commercial IrO2-based anodes at 50◦C. (e) Long-term stability of a-NiFeOOH/N-CFP electrode in electrolyzer with a constant cell voltage of 2.0 V for 10 days (g) Experimental and theoretical hydrogen yields (Faradaic efficiency) calculated through water displacement system (Thangavel et al.,2021).
an operating current density of 1 A/cm2 with∼80% energy ef- ficiency. Furthermore, long-term stability is studied at constant voltage of 20.V for 240 h continuously where the prepared 3D- a-NiFeOOH/N-CFP electrode exhibited stability retention of 95.6%
with ultra-low degradation rate of 0.15 mA h−1and the Faradaic efficiency of 98.5%.
Guo et al.(2021) reported the facile and rapid synthesis of Cu- Co-P on carbon paper (CP) substrate using the electrodeposition technique. Initially, Co-P/CP deposition conditions are optimized and studied for HER in alkaline solution, the attained results showed acceptable electrocatalytic activity with an overpotential of 72 mV at a current density of 10 mA cm−2. Further modified the surface properties including the electronic structure and in- creased the active sites of Co-P by incorporating Cu for enhancing the electrochemical performance. The modified Cu-Co-P1200/CP exhibited superior performance with an ultra-low overpotential
of 59 mV at a current density of 10 mA cm−2 and a smaller Tafel slope of 38 mV dec−1, as shown inFig. 8. Moreover, the synthesized Cu-Co-P1200/CP performance studied towards the hydrogen evolution reaction as a cathode electrode in a single cell AEM water electrolyzer with an anode material of commercial IrO2/CP, the achieved cell voltage of 1.9 V at an operating current density of 0.70 A cm−2with good stability, which is slightly lower than that of noble metal-based electrodes of Pt/C/CP@IrO2/CP. But this performance is superior to those in literature for non-noble metal-based electrodes.
Further,Jang et al.(2020a,b) synthesized a noble metal-free nanosized Cu0.5Co2.5O2anode electrocatalyst via co-precipitation technique by adjusting the pH for AEM water electrolysis and studied their performance in alkaline solution as well as water electrolyzer.
The synthesized Cu0.5Co2.5O2 electrode exhibited improved electrochemical performance with an overpotential of 285 mV
Fig. 8. (a) HER polarization curves of Cu-Co-P1200/CP electrodes with different concentrations of Cu2+in 1M KOH solution with scan rate of 5 mV s−1(b) (e) effect of Cu2+concentration on overpotential at constant current density of 10 mA/cm2 (c) Tafel slopes (d) Current–Voltage polarization cures of single cell AEM water electrolyzer with IrO2/CP as anode coupled with as synthesized Cu10-Co-P1200/CP electrode as cathode and compared with the commercial Pt/C/CP (Guo et al.,2021).
at 10 mA cm−2 in 1M KOH solution. Further, the developed Cu0.5Co2.5O2electrocatalyst performance was studied in a single- cell with the active area of 4.9 cm2 AEM water electrolyzer as an anode and commercial Pt/C used as a cathode, the archived current density of 1.3 A cm−2 at 1.8 V at 45 ◦C with 1M KOH solution. Furthermore, durability studies were carried out for 100 h continuously at a constant current density of 400 mA cm−2it maintained 80% energy efficiency during 100 h operation.
In addition, demonstrated excellent stability at constant current density of 10 mA cm−2 for 2000 h. Chen et al. (2021) devel- oped poly (fluorenyl-co-aryl piperidinium) (PFAP)-based anion exchange materials i.e., membrane electrolyte and binder with high ionic conductivity and durability under alkaline media. The developed electrolyte with platinum group metal (PGM) catalysts (IrO2 and Pt/C) achieved a new record cell performance of 7.68 A/cm2 at 2 V with 1M KOH and PGM-free materials (Ni-Fe) displayed an outstanding current density of 1.62 A cm−2 at 2.0 V. Additionally, PGM and PGM-free materials displayed excellent durability of more than 1000 h of operation at the constant current density of 0.5 A cm−2 at 60 ◦C without any voltage degradation.
3.3. PEM water electrolysis
To overcome the drawbacks of alkaline water electrolysis, the 1st PEM water electrolysis phenomenon was idealized by
Grubbs and developed by General Electric Co. in the year of 1966 (Shiva Kumar and Himabindu,2019a). However, PEM water elec- trolysis technology is similar to the PEM fuel cell technology, here the sulfonated polymer membrane can be used as an electrolyte.
The ionic charge carrier is H+and DI water permeating through the proton-conducting membrane it provides the functionality of the electrochemical reaction. Typically, PEM water electrolysis operates at lower temperatures (30–80◦C) with higher current densities (1–2 A/cm2) and produces high purity (99.999%) of gases (Hydrogen and Oxygen) (Shiva Kumar and Himabindu, 2019a).
Because the kinetics of hydrogen evolution reaction in PEM wa- ter electrolysis is faster than alkaline water electrolysis due to the highly active area of the metal surface of Pt electrodes and lower pH of the electrolyte. In addition, PEM water electroly- sis is safer than alkaline water electrolysis due to the absence of caustic electrolytes and smaller footprint. Therefore, globally several water electrolyzer manufacturers (listed inTable 4) are developed large-scale (up to MW) PEM water electrolyzers for industrial and transportation applications. The reported stability of PEMWE is 60,000 h with negligible loss of performance and the targeted stability is 1,00,000 h (Schmidt et al.,2017;Wei et al., 2019). However, the major challenges associated with the PEM water electrolysis are high cost of the components i.e., electrode materials, current collectors, and bipolar plates respectively.
Fig. 9. Schematic view of PEM water electrolysis working principle.
3.3.1. Working principle of pem water electrolysis
During the PEM water electrolysis process, water is electro- chemically split into hydrogen and oxygen. In this process, ini- tially at the anode side water molecule is decomposed to generate oxygen (O2) and protons (H+), and electrons (e−). The generated oxygen eliminated from the anodic surface and the remaining protons are traveled through the proton-conducting membrane to the cathode side and the electrons are traveled through the external circuit to the cathode side. At the cathode side, the protons and electrons recombined to produce H2 gas. The basic principle of PEM water electrolysis is shown inFig. 9.
3.3.2. Cell components of PEM water electrolysis
The PEM water electrolysis cell major components are mem- brane electrode assembly (consist of membrane and anode, cath- ode electrode materials), Gas diffusion layer, separator plates (bipolar plates), and end plates respectively (Shiva Kumar et al., 2018c; Shiva Kumar and Himabindu, 2019a; Upadhyay et al., 2020,2022). Typical proton exchange membranes are Nafion®, Fumapem®, Flemion®, and Aciplex® respectively. However, most widely used membrane is Nafion® (Nafion® 115, 117, and 212), because Nafion®membrane offers several advantages such as high proton conductivity, possess high current density, high mechanical strength, and chemical stability respectively.
The state-of-the-art anode and cathode electrode materials are noble metal based electrocatalysts especially IrO2 for the OER and carbon-supported Pt for the HER respectively (Ramakrishna et al.,2016;Shiva Kumar et al.,2018a,d;Lee et al.,2019). These noble metals are more expensive, and iridium is scarcer than plat- inum. For example, a 10 MW PEM water electrolyzer operating at 1 A/cm2 requires about 15 kg of Iridium with an assumed catalyst loading of 2–3 mg/cm2, the expected cost of Iridium catalyst would be more than 2,941,789 US$ (196,119 US$/kg in August 2021) (Metalary, 2021). The porous titanium/titanium mesh and carbon cloth are used as anode and cathode gas dif- fusion layers. Different flow field designed bipolar plates made up of titanium material coated with platinum/gold are used as separators and endplates respectively. Among different flow field designs, the straight parallel flow field designed separator plates have shown better performance, especially in PEM water electrolyzer (Yang et al.,2019). However, these separator plates are expensive and are responsible for 48% of the overall cell cost (IRENA,2020b). Therefore, the cost-effective cell components i.e., electrode materials and separator plates still under challenge.
3.3.3. Research and development of pem water electrolysis
PEM water electrolysis technology is well developed and com- mercially available up to megawatt (MW) for industrial and trans- portation applications, some of the large-scale PEM electrolyzer manufacturers are listed inTable 4. However, several improve- ments are still required to reduce the hydrogen production cost, the present hydrogen production cost is USD 700–1400 kW/H2 (2020), and targeted cost reduction is USD≤200 kW/H2 (2050) (IRENA, 2020b). To achieve this target, the existing challenges need to be addressed such as replacement/reduction of platinum group metals with cost-effective transition metals, removing the expensive coatings on bipolar plates, and redesigning the new bipolar plates with cost-effective materials. Moreover, to reduce the membrane thickness and enhance the cell efficiency. Cur- rently, the Nafion®117 (thickness 180µm) membrane is using in PEM water electrolyzers, the efficiency loss from this membrane is 25% (at 2 A/cm2), if reducing the thickness as low as 20 µm the predicted reduction efficiency losses is 6% (at 2 A/cm2).
Therefore, in this direction several researchers from public and private organizations are still working on their developments especially focusing on cost reduction. For example, Xie et al.
(2021) reported integrated electrode architectures to consist of platinum nanowires on ultrathin titanium gas diffusion layers for hydrogen evolution reaction in PEM water electrolysis. The ultrathin titanium integrated PtNW electrode (PtNW/Ti) showed a lower overpotential of 63 mV at the higher current density of 100 mA cm−2with a smaller Tafel slope of 35 mV dec−1. Further, electrochemical performances were studied in PEM water elec- trolyzer as a cathode electrode, the attained results demonstrated that the PtNW/Ti electrode has showed a lower cell voltage of 1.643 V at 1 A cm−2 and high efficiency of 90.08% with 15 times lower catalyst loadings than conventional MEAs in PEM water electrolysis. Also, Xie et al. (2022) developed ionomer- free integrated electrodes (1T-2H MoS2NS/CFP) using engineered 1T-2H heterophase with MoS2 nanosheets (MoS2NSs) by in-situ growing on carbon fiber paper with MoS2 loading of only 0.14 mg/cm2 for HER and studied their performance in 0.5M H2SO4 as well as in PEM water electrolyzer. The integrated electrode has shown outstanding performance with an extremely lower overpotential of 192 mV and a smaller Tafel slope of 44 mV dec−1. Further, the PEM water electrolyzer results exhibited that, the integrated electrode impressively achieved a cell voltage of 2.25 V at an operating current density of 2 A/cm2, as shown in Fig. 10. Furthermore, the integrated electrode performance was
Fig. 10. Schematic illustration of Ionomer-free electrode with in-situ grown ultralow-loading and defect-rich 1T-2H MoS2 nanosheets. (a–f) HAADF-STEM images of defect-rich 1T-2H MoS2NS/CFP, confirming the co-existence of edges, pinholes & atomic vacancies. (g) Polarization curves of defect-rich 1T-2H MoS2NS/CFP and MoS2 assemblies/CFP. (h) Corresponding Tafel plots. (i) Polarization curves of defect-rich 1T-2H MoS2NS/CFP and MoS2 assemblies/CFP in a PEMEC at 80 ◦C (Xie et al.,2022).
compared with the commercial Pt/C catalysts with similar metal loading of 2.0 mg/cm2. The commercial Pt/C catalyst exhibited a lower cell voltage of 2.18 V than that of the integrated 1T-2H MoS2NS/CFP electrode (2.25 V) at the current density of 2 A cm−2 but this performance is superior to reported non-noble catalysts.
Jang et al. (2020a,b) introduced a novel titanium-doped molybdenum phosphide (Ti-MoP) electrocatalyst for hydrogen evolution reaction in acid electrolyte. The developed Ti-MoP elec- trocatalyst demonstrated superior electrochemical performance than undoped MoP with an overpotential of only 81.5 mV at 10 mA cm−2than that of undoped MoP (93.5 mV) under the acidic electrolyte (0.5M H2SO4), indicating that the HER performance is improved approximately 13% by doping Ti with MoP. The Tafel slope also shows that Ti-MoP has a lower (44.5 mV dec−1) than that of undoped (MoP 46.3 mV dec−1). Further, the electro- chemical stability was studied for 8000 cycles and 15 days for undoped MoP and Ti-doped MoP, the Ti-doped MoP electrocat- alyst exhibited improved stability in 0.5M H2SO4solution.Yoon et al.(2021) developed a platinum-free cobalt phosphide (Co-P) electrode for the hydrogen evolution reaction, the electrode was fabricated on carbon paper by pulse electrodeposition technique with various dissolution amounts of Co. The acid-dissolved Co- P-0.3 electrode showed better electrochemical performance with an overpotential of 143.85 mV at the current density of 10 mA cm−2and the Tafel slope of 60.10 mV dec−1. Further, the single- cell water electrolysis experiments were also carried out with Co-P-0.3 as a cathode electrode, which showed the remarkable performance, the achieved current density of 1.89 A cm−2 at a cell voltage of 2.0 V.Tajuddin et al.(2021) reported noble metal- free graphene-encapsulated NiMo alloy as an acid-stable catalyst for HER. The N-doped graphene (4–8 layers) encapsulated NiMo cathode catalyst exhibited an extremely stable electrochemi- cal performance in the potential cycling test of 10,000 cycles.
Moreover, exhibited highly stable electrochemical performance after the 100 h of stability test at the constant cell voltage of 2.2 V in single cell PEM water electrolyzer. Recently,Atchudan et al.(2022) developed a noble metal-free molybdenum disulfide decorated banana peel porous carbon (MoS2@BPPC) catalyst for hydrogen evolution reaction (HER). The developed MoS2@BPPC composite electrocatalyst showed higher HER activity and pos- sessed superior stability in the acidic conditions (0.5M H2SO4) with an overpotential of 150 mV at the current density of 10 mA cm−2, and the Tafel slope of 51 mV dec−1. Further,Brito et al.
(2022) introduced transition metal phosphide catalyst supported on carbon black (FeP/CB) for HER as an alternative to platinum- based catalysts. The prepared 50% FeP/CB catalyst showed better electrocatalytic activity with an achieved overpotential of 252 mV at the current density of 10 mA cm−2, which is quite close to the 220 mV of platinum catalyst.
Jiang et al.(2021) designed Ir film decorated WOx nanorods (Ir@WOxNRs) through electrodeposition techniques for OER elec- trodes and studied their electrochemical performance in acidic media. The designed Ir@WOxNRs electrode with reduced no- ble metal loading of 0.14 mg cm−2 demonstrated outstanding electrochemical performance and stability, the achieved current density of 2.2 A cm−2at 2 V with an acceptable degradation rate of 49.7µV h−1during the 1030 h stability test at a constant cur- rent density of 0.5 mA cm−2. Further,Jiang et al.(2022) developed WO3 nano-array electrode with a heterogeneous IrRu coating with different Ir/Ru ratios by facile electrodeposition approach and studied their OER activity and stability in acidic conditions.
The developed Ir3.2Ru1.6@WO3 electrode exhibited outstanding electrocatalytic activity and stability with a competitive overpo- tential of 245 mV at 10 mA cm−2, which is lower than that of commercial IrO2 (290 mV). Further, the single cell PEM water electrolysis results were exhibited an extremely high current